|Year : 2020 | Volume
| Issue : 7 | Page : 950-956
Evaluating efficacy of different post materials and lengths on bonding strength between root canal dentin and post restorations: An experimental study
M Ulgey1, R Zan2, O Gorler1, G Yesilyurt1, F Cotur2
1 Department of Prosthodontics, Faculty of Dentistry, Sivas Cumhuriyet University, Sivas, Turkey
2 Department of Endodontics, Faculty of Dentistry, Sivas Cumhuriyet University, Sivas, Turkey
|Date of Submission||06-Sep-2019|
|Date of Acceptance||21-Feb-2020|
|Date of Web Publication||3-Jul-2020|
Dr. M Ulgey
Department of Prosthodontics, Faculty of Dentistry, Sivas Cumhuriyet University, Sivas
Source of Support: None, Conflict of Interest: None
| Abstract|| |
Background: During post restoration, different root structures require several types of posts to increase duration of their clinical use. Several materials have been investigated to enhance their quality and optimize their length according to the available root canal. Aims: The aim of this study was to determine the effect of zirconia, fiber, and ceromer posts with 3- and 6-mm post sizes on the bonding strength of them to root canal dentinal wall with the means of pull-out bond strength test. Methods: Forty-eight single-rooted mandibular human premolar teeth were collected and prepared for this in vitro study. With resin cement, 3- and 6-mm study posts including zirconia, fiber, and ceromer were luted to prepare teeth. For the retention testing, the pull-out force was applied to each specimen parallel to longitudinal axis of both the post and tooth. Results: Both type of materials and size of posts changed the value of bonding strength. In all the post types, 6-mm ones performed better. Overall, the best bonding strength was obtained with fiber posts and the better bonding strength was obtained with zirconia; however, ceromer provided the least bonding strength. Conclusion: Current experiments supported that 6-mm post size can increase the bonding between root canal dentin and studied posts. When considering post materials, fiber provided the best bonding strength in current laboratory setup. Second, zirconia had meaningfully acceptable bonding strength; however, the bonding strength of ceromer posts was not favorable. Further studies optimizing post fabrication techniques of root materials may increase the bonding strength of posts to human dentin to an acceptable clinical degree.
Keywords: Dental prosthesis retention, dentin, post and core technique, shear force
|How to cite this article:|
Ulgey M, Zan R, Gorler O, Yesilyurt G, Cotur F. Evaluating efficacy of different post materials and lengths on bonding strength between root canal dentin and post restorations: An experimental study. Niger J Clin Pract 2020;23:950-6
|How to cite this URL:|
Ulgey M, Zan R, Gorler O, Yesilyurt G, Cotur F. Evaluating efficacy of different post materials and lengths on bonding strength between root canal dentin and post restorations: An experimental study. Niger J Clin Pract [serial online] 2020 [cited 2021 Jun 12];23:950-6. Available from: https://www.njcponline.com/text.asp?2020/23/7/950/288879
| Introduction|| |
Retention of coronal structure and health of periodontal tissues should be provided with the restoration of root-filled teeth., If more than 50% part of the coronal structure is damaged, post application is required to provide extra strength to the tooth. Remaining coronal tooth tissue is mostly insufficient for supporting the restoration in anterior and premolar teeth without post applications. The selection of post is dependent on the remaining root, its size, and shape. For decades, cast metal posts have been used for treating of root-filled teeth. Even though these conventional posts have high retention and thin resulting cement film, they have a high elastic modulus and can result in root fractures. Similar elastic modulus of fiber posts, resin cements, and dentin is beneficial to enhance the performance of restorations. The advantages of ceramics and reinforced resins compared to metal alloys are the elimination of galvanic corrosion  and decrease of toxicity of metallic ions.,
Production method, material type, and size of the post are important factors for the retention., Optimal preparation of post space is essential to achieve adequate retention. The remaining short and curved root restricts the use of a longer dowel.In vitro studies have revealed that cements reinforced with resin may be used to tolerate reduction of the length. For the prosthetic treatment of root-filled teeth with major hard tissue loss, the use of fiber posts and self-adhesive resin cement is a popular treatment solution. In scientific literature, many studies have revealed that the successful clinical results of fiber posts were associated with mechanical stress and their superior retention values., Elasticity modulus of fiber post and dentin are alike (resp., 18–22 GPa and 18 GPa); thus, this material is used to reduce the risk of root fracture.,
Zirconia posts are tooth-colored materials and generally used in anterior teeth for esthetic reasons. Commercially available prefabricated zirconia posts may be preferred by the clinicians for the treatment of root-filled teeth. In addition, for the increasing the strength of the teeth with wide root canals, one-piece zirconia posts can be manufactured with CAD/CAM technology after taking impression from the root canal. Zirconia posts have some advantages including greater resistance, greater toughness, and adequate esthetics., However, elasticity modulus of zirconia material is not similar with dentin. This is a disadvantage of zirconia material that can cause vertical root fracture because of transmitting the chewing force directly from zirconia post to the root canal. There are ceramic optimized resins/polymers (ceromers) among the advanced types of composite materials. The properties of ceramic fillers are also used to enhance the physical and mechanical properties of composites like improved mechanical strength and abrasion resistance.,
Survival of post restorations depends on retention to the root canal. Loss of retention is primary failure mode for post restorations and this was shown in both in vivo and in vitro studies.,, However, there is still no consensus on the type of post regarding its material and size that can provide more superior long-term clinical retention of post-retained restorations. It was thought that dentinal wall needs to be improved with the investigation of suitable materials and the optimal size of posts in order to improve the bonding strength of posts to root canal. The purpose of this study was to assess the effect of zirconia, fiber, and ceromer posts with 3- and 6-mm post sizes on their bonding strength to root canal dentinal wall by pull-out bond strength test. The null hypothesis was that the pull-out strengths of zirconia, fiber, and ceromer with different post sizes to root dentin surface were similar.
| Material and Methods|| |
Approval from the Human Research Ethics Committee of our university was obtained (No: 2019-08/17). In this in vitro study, forty-eight single-rooted mandibular human premolar teeth that extracted with orthodontic or periodontal indications without any caries or previous restorations were used. Digital radiographs of teeth were taken from the buccal and proximal directions to determine the number and morphology of their canals. After dental plaque, calculus, and periodontal tissues were cleaned, they were kept at + 4°C in 0.9% saline solution during the whole study. The coronal part of the tooth was cut using diamond discs below the level of the cemento-enamel junction under cooling water to obtain a 14-16 mm length for each root. First, a 15-number K-File (Mani Inc., Japan) hand tool was used to enter the canal. Working length of the canal was determined by transmitting the file until it can be seen in the apical foramen. Then, the file was withdrawn 1 mm from the apex. Root canal preparation was performed with Protaper Universal (DentsplyMaillefer, Switzerland) system according to the crown-down technique by using an electric motor (Dentaports ZX, J. Morita Mfg. Corp., Japan). The root canals were irrigated with 1 mL of 5.25% NaOCl solution after the use of each file. Then, root canals were dried with paper points. Afterward, they were filled with lateral condensation technique using AH Plus (DentsplyMaillefer, Switzerland) and gutta-percha. For the preparation of post space, gutta-percha in the root canal was removed and space was created with a size #3 fiber post drill (D.T Light-Post, Bisco Inc., USA) for two post lengths: 3 mm and 6 mm.
For the production of zirconia post, 3D shape of post space was captured with light body (Elite HD+, ZhermackSpA, Italy) and putty (Elite HD+, ZhermackSpA, Italy) polyvinyl-siloxane impression materials. Light-body impression material was delivered into the post hole and a plastic-post was used as a carrier for this impression. The putty material was prepared by hand and applied to coronal part of the post restoration for facilitating its removal. After setting of the impressions, they were removed from the post space by ensuring that it extends to end of the prepared post space, it will not lock into any undercut, and it is free of any voids or defects. For digitalizing the impression, contrast spay (Calidia, Whitepeaks Dental Solutions Inc., Germany) was applied to the impression and scanned with model scanner (Dental Wings 7 Series; Dental Wings, Canada). Post and core structures were designed in software (DWOS, Dental Wings, Canada) [Figure 1] and [Figure 2] and subtracted from pre-sintered Y-TZP disc-shaped block (ST, Upcera, China) by using milling machine (DC40, Yenadent, Turkey). After computer-aided design (CAD) and computer-aided manufacturing (CAM) process, the samples were sintered to full density in a high-temperature furnace (Protherm; B and D Dental Origin Milling, USA) at 1480°C for 2 h according to the manufacturer's instructions [Figure 3].
For the production of ceromer post, individual molds were prepared for 3 mm and 6 mm groups separately using polyvinyl-siloxane impression material. For the preparing of individual mold, a fiber post was measured with scale (Endoring II, JordcoInc, USA) and placed into impression material before set of the impression. After setting, fiber post material was carefully removed from the impression; thus, appropriate space for the production of ceromer post was created. Then, ceromer material was placed into space and carefully adapted with a hand instrument (OP2X, Optident Ltd, UK). Ceromer material was polymerized for 20 s with a light-curing device for removing easily from the mold. After they were removed from the mold, they were subjected to a polymerization process according to manufacturer's instructions. First, ceromer posts were polymerized by Light Curing-300 device for 270 s. Then, final polymerization was performed with Heat-Curing-110 furnace for 15 min at 100°C–110°C.
After preparation of all post restorations, they were cleaned by using 95% ethyl alcohol and air-drying. For the cementation, a self-adhesive resin cement (G-Cem, GC Corp., Japan) was delivered into the post space with a lentulo spiral (Mani Inc., Japan). Post restorations were seated to post hole and held under moderate finger pressure for 10 s. The excess cement was gently removed using microbrush after the posts-core restorations were completely seated. The surfaces were light-cured for 40 s with a light-emitting diode light polymerizing unit (Smartlite, Dentsply, USA).
For pull-out testing, each specimen prepared for the study was embedded in autopolymerizing dental acrylic (Meliodent, Heraeus Kulzer, Germany) in aluminum cylinders with a diameter of 14 mm and a height of 12 mm. Thereafter, the specimens were stored in distilled water for 1 week at 37°C. For the retention testing, the pull-out force was applied to each specimen parallel to longitudinal axis of both the post and tooth by a universal test machine (Lloyd LF Plus, AmetekInc, UK) with a cross-head speed of 2 mm per minute. Maximum tensile force (N) was recorded for each specimen.
The data were expressed as mean ± SD. Statistical analysis of the data was performed using a Kolmogorov-Smirnov test to examine normality and then a one-way analysis of variance, Tukey post hoc tests, and t-test to compare the pull-out bonding strength data. A P value of less than 0.05 was used to describe significant differences.
| Results|| |
[Figure 4] presents the values of pull-out bonding strength of zirconia, fiber, and ceromer posts sized 3 and 6 mm. ANOVA and t tests revealed that overall bonding strengths of studied specimens were significantly different. Both type of materials and size of posts changed the value of bonding strength. The bonding strength of 6-mm zirconia post was significantly higher than the bonding strength of the 3-mm zirconia post (8.40 ± 0.22 vs. 7.73 ± 0.20; P < 0.05). The bonding strength of the 6-mm ceromer post was significantly higher than the bonding strength of the 3-mm ceromer post (7.48 ± 0.21 vs. 7.10 ± 0.14; P < 0.05). Although the bonding strength of the 6-mm fiber post was higher than the bonding strength of the 3-mm fiber post, this difference was not statistically significant (8.75 ± 0.19 vs. 8.55 ± 0.17; P > 0.05).
|Figure 4: Values of pull-out bonding strength of zirconia, fiber, and ceromer posts sized 3 and 6 mm. The data were expressed as mean (midline) and SD (whiskers). aP < 0.05, 6-mm zirconia post vs. 3-mm zirconia post. bP < 0.05, 6-mm ceromer post vs. 3-mm ceromer post. cP < 0.05, 3-mm fiber post vs. 3-mm zirconia post. dP < 0.05, 3-mm zirconia post vs. 3-mm ceromer post. eP < 0.05, 3-mm fiber post vs. 3-mm ceromer post. fP < 0.05, 6-mm zirconia post vs. 6-mm ceromer post. gP < 0.05, 6-mm fiber post vs. 6-mm ceromer post|
Click here to view
The pull-out bonding strength test revealed that there was a significant difference between 3-mm fiber and zirconia posts regarding the bonding strength values (8.55 ± 0.17 vs. 7.73 ± 0.2; P < 0.05). The bonding strength of the 3-mm zirconia post was significantly higher than that of the 3-mm ceromer post (7.73 ± 0.2 vs. 7.10 ± 0.14; P < 0.05). The 3-mm fiber post had significantly higher bonding strength compared to the 3-mm ceromer post (8.55 ± 0.17 vs. 7.10 ± 0.14; P < 0.05). The bonding strength of the 6-mm zirconia post was significantly higher than the bonding strength of the 6-mm ceromer post (8.40 ± 0.22 vs. 7.48 ± 0.21; P < 0.05). The 6-mm fiber post provided a significant increase in the bonding strength compared to the 6-mm ceromer post (8.75 ± 0.19 vs. 7.48 ± 0.21; P < 0.05). Although the bonding strength of the 6-mm fiber post was higher compared to the 6-mm zirconia post, this difference was not statistically significant (8.75 ± 0.19 vs. 8.40 ± 0.22; P > 0.05).
| Discussion|| |
Our null hypothesis was not confirmed by the bonding strength data of the present in vitro study. The bonding strength data obtained with the pull-out test supported that the size of post was important to increase the bonding strength of zirconia, fiber, and ceromer materials to the root canal. In accordance with the increase of post size, there was an increase in the bonding strength. When considering the studied post materials of zirconia, fiber, and ceromer, significant differences were found between the bonding strength of posts prepared with these materials. The most favorable results in bonding strength measurements were obtained with fiber posts. Second, the considerably good results in bonding strength measurements were found with zirconia. The least favorable results in bonding strength measurements were recorded with ceromer. According to the type of material and the size of post, the optimal type of post was designed as 6-mm fiber post.
When considering specimen preparation methods used in this study, there may be some limitations in these experiments. During the preparation of fiber posts, a commercial set of fiber was used for post preparation. It was thought that this may help the optimization of adaptation between the post and root canal dentin. On the other hand, for the preparation of zirconia and ceromer posts, we need to use post preparation techniques as mentioned in the Methods. These specimen preparations may decrease the optimization of adaptation between the posts and root canal dentin. In further studies, analysis of space between post and root canal dentin by microscopy modalities and association of this finding with the bonding strength may shed light on the difference of bonding values of currently studied posts.
During post restoration in clinical practice, it is not easy to obtain a desired post length as suggested two-thirds of the root in some of the cases. In addition, the post size necessary based on the tooth anatomy  and preventive measures should be taken into account during the process of post space preparation. The results of the study by Holmes et al. supported that the stress peak was observed adjacent to the post and increased by 57% when post length decreased from 13 mm to 8 mm. On the other hand, Yang et al. stated that the stresses in the apical region increased when dowel length increased beyond two-thirds of the root and they suggested that extension of post length may be harmful to the root apical sealing. When considering the implications of those studies, there is a need to pay attention to maintain an apical seal of 4 to 5 mm of gutta-percha. Braga et al. suggested that in the presence of short and curved roots, it is logical to select an 8-mm post since they found no significant difference between 8- and 10-mm posts.
Christel et al. observed that zirconia posts, introduced in the late 1980s, exhibited high resistance to fractures; additionally, Kwiatkowski and Geller  revealed that zirconia post can be used as bonded with a resin cement. This can be related to the smooth surface of zirconia after sinterization but this condition can be a negative contributor for the bonding quality of zirconia and resin cement. In a pertinent study, Al-Harbi and Nathanson  measured the retentive strength between composite and ceramic endodontic dowel systems and the tooth and its fabricated core. According to their results, the ceramic dowel systems were not successful compared to other studied system regarding bonding values. Concerning improvement of the bonding quality of ceramic posts, Kakehashi et al. indicated a positive effect of airborne-particle–abrasion on the post surface to improve bonding level. In the current study, we did not use this technique, because of possible phase transformation of zirconia and its detrimental effect on its structure.,
Contrary to the results of the present study, Bottino et al. conducted a study to determine the effect of cyclical mechanical loading on bond strength of a fiber and a zirconia post bonded to root dentin. In their study, the push-out bonding strength of zirconia post was higher compared to the fiber post but this difference was not significant. In the current study, we fabricated the zirconia post in the laboratory; however, in their study, zirconia specimens were prefabricated. This may be the cause of difference between the results of the study by Bottino et al. and the present study.
Properties of fiber posts such as having elasticity modulus similar with dentin, greater retention values to root canal, and adequate esthetic properties can be related to the success with their long-term clinical use. In the pertinent literature, there are several studies presenting the positive association of post length and retention ,,,,, The results of Nergiz et al. supported that dowel length was the most important factor for the retention of post compared to dowel diameter. They noted that this might be related to the increased surface area of the post. Another study also revealed similar results after artificial aging.
In the literature, there are studies presenting results supporting the potential clinical use of short post., The fact that the bonding performance of cement is more effective in cervical third than in the apical third may be the cause of advantage during the use of fiber posts for short roots or roots having a high degree of curvature. Webber et al. stated that the preparation of 1/2 of the remaining root can be preferred when 2/3 of the preparation of the remaining root was not performed. Borer et al. explained that 10-mm posts requiring greater force to dislodge than their 5-mm counterparts also provided adequate retention.
During fabrication of ceromer material, different fillers to reinforce polymers, as an inorganic–organic hybrid polymeric material, can be used. These fillers can improve wear resistance and lifespan of these composites with the support of increased mechanical strength and abrasion resistance.,
In the present study, it was thought that it is possible to use ceromer as a test material for post development. For this purpose, some properties of ceromer can be helpful when they were used as a post material, including its content as polymer structure similar to that of resin cement and their potential compatibility; flexible structure reducing vertical root fracture; and tooth-colored surface increasing patient's satisfaction. However, in the current laboratory settings, ceromer was not performed well compared to other studied materials. This may be the result of complicated fabrication technique used in our laboratory.
In our laboratory setup, the pull-out bond strength test was preferred because it is a reliable and validated method of evaluating the performance of post specimens to resist shearing stresses. During this test, with applied forces, the stress was distributed better on the surface of post and this may increase the precision of measurements. When posts have higher retention with pull-out test, they are more resistant to dislodgement as a result of lateral occlusal stresses.,
The main idea of the present study was to include a variety of post materials including zirconia, fiber, and ceromer, to simulate clinically relevant conditions of post restoration, and to explore if the bonding strength between root canal dentin and customized zirconia, fiber, and ceromer posts would also be affected by different sizes of posts. Current experiments supported that post material and size can increase the bonding between root canal dentin and studied posts. In addition, to the best of authors' knowledge, this is the first attempt to measure the bonding strength of these materials with different sizes by pull-out test in the same laboratory settings, and the current experiments provided in vitro data about the suitability of ceromer as post material. Further studies may be helpful to explore the effect of their different sizes to optimize the potential merit of fiber posts for use during post restorations.
| Conclusion|| |
Based on the limitations of the present study, the following conclusions may be reached:
- The bonding strength of the 6-mm zirconia, fiber, and ceromer posts was significantly higher compared to their 3-mm pairs.
- The bonding strength of the 3- and 6- mm fiber posts was significantly higher compared to the 3- and 6-mm zirconia and ceromer posts.
- The 3- and 6-mm ceromer posts provided the lowest values of bonding strength compared to other post types.
The authors thank Zhermack SpA, Italy, for donating the disinfection material used in this study. The authors have no commercial relationships to declare.
Financial support and sponsorship
Conflicts of interest
There are no conflicts of interest.
| References|| |
Chang J, Soo I, Cheung GS. Evaluation of fiber post-supported restorations under simulated occlusal loading. J Prosthet Dent 2012;108:158-64.
Zicari F, Van Meerbeek B, Scotti R, Naert I. Effect of fibre post length and adhesive strategy on fracture resistance of endodontically treated teeth after fatigue loading. J Dent 2012;40:312-21.
Alsamadani KH, Abdaziz E-SM, Gad E-S. Influence of different restorative techniques on the strength of endodontically treated weakened roots. Int J Dent 2012;2012:343712.
Cheung W. A review of the management of endodontically treated teeth: Post, core and the final restoration. J Am Dent Assoc 2005;136:611-9.
Webber MBF, de Araújo Michida SM, Marson FC, de Oliveira GC, e Silva CdO. Analysis of bond strength by pull out test on fiber glass posts cemented in different lengths. J Int Oral Health 2015;7:7.
Dietschi D, Duc O, Krejci I, Sadan A. Biomechanical considerations for the restoration of endodontically treated teeth: A systematic review of the literature, Part II (Evaluation of fatigue behavior, interfaces, and in vivo
studies). Quintessence Int 2008;39:117-29.
Schmitter M, Huy C, Ohlmann B, Gabbert O, Gilde H, Rammelsberg P. Fracture resistance of upper and lower incisors restored with glass fiber reinforced posts. J Endod 2006;32:328-30.
Bergman M, Bergman B, Söremark R. Tissue accumulation of nickel released due to electrochemical corrosion of non-precious dental casting alloys. J Oral Rehabil 1980;7:325-30.
Bearden L, Cooke F. Growth inhibition of cultured fibroblasts by cobalt and nickel. J Biomed Mater Res 1980;14:289-309.
Jacobsen N. Epithelial-like cells in culture derived from human gingiva: Response to nickel. Eur J Oral Sci 1977;85:567-74.
Galhano GA, Melo RM, Pavanelli CA, Baldissara P, Scotti R, Valandro LF, et al
. Adhesive cementation of zirconia posts to root dentin: Evaluation of the mechanical cycling effect. Braz Oral Res 2008;22:264-9.
Gernhardt CR, Bekes K, Schaller H-G. Short-term retentive values of zirconium oxide posts cemented with glass ionomer and resin cement: An in vitro
study and a case report. Quintessence Int 2005;36:593-601.
Holmes DC, Diaz-Arnold AM, Leary JM. Influence of post dimension on stress distribution in dentin. J Prosthet Dent 1996;75:140-7.
Sen D, Poyrazoglu E, Tuncelli B. The retentive effects of pre-fabricated posts by luting cements. J Oral Rehabil 2004;31:585-9.
Akkayan B, Gülmez T. Resistance to fracture of endodontically treated teeth restored with different post systems. J Prosthet Dent 2002;87:431-7.
Grandini S, Goracci C, Monticelli F, Tay FR, Ferrari M. Fatigue resistance and structural characteristics of fiber posts: Three-point bending test and SEM evaluation. Dent Mater 2005;21:75-82.
Asmussen E, Peutzfeldt A, Heitmann T. Stiffness, elastic limit, and strength of newer types of endodontic posts. J Dent 1999;27:275-8.
Lassila LV, Tanner J, Le Bell A-M, Narva K, Vallittu PK. Flexural properties of fiber reinforced root canal posts. Dent Mater 2004;20:29-36.
Michalakis KX, Hirayama H, Sfolkos J, Sfolkos K. Light transmission of posts and cores used for the anterior esthetic region. Int J Periodontics Restorative Dent 2004;24:462-9.
Heydecke G, Butz F, Hussein A, Strub JR. Fracture strength after dynamic loading of endodontically treated teeth restored with different post-and-core systems. J Prosthet Dent 2002;87:438-45.
Awad MA, Marghalani TY. Fabrication of a custom-made ceramic post and core using CAD-CAM technology. J Prosthet Dent 2007;98:161-2.
Streacker AB, Geissberger M. The milled ceramic post and core: A functional and esthetic alternative. J Prosthet Dent 2007;98:486-7.
Ichikawa Y, Akagawa Y, Nikai H, Tsuru H. Tissue compatibility and stability of a new zirconia ceramic in vivo
. J Prosthet Dent 1992;68:322-6.
Zanghellini G. Fiber-reinforced framework and Ceromer restorations: A technical review. Signature 1997;4:1-5.
Khan AS, Azam MT, Khan M, Mian SA, Rehman IU. An update on glass fiber dental restorative composites: A systematic review. Mater Sci Eng C 2015;47:26-39.
Cantoro A, Goracci C, Vichi A, Mazzoni A, Fadda GM, Ferrari M. Retentive strength and sealing ability of new self-adhesive resin cements in fiber post luting. Dent Mater 2011;27:e197-204.
Mastoras K, Vasiliadis L, Koulaouzidou E, Gogos C. Evaluation of push-out bond strength of two endodontic post systems. J Endod 2012;38:510-4.
Sahafi A, Peutzfeldt A, Asmussen E, Gotfredsen K. Retention and failure morphology of prefabricated posts. Int J Prosthodont 2004;17:307-12.
Sokol DJ. Effective use of current core and post concepts. J Prosthet Dent 1984;52:231-4.
Nergiz I, Schmage P, Özcan M, Platzer U. Effect of length and diameter of tapered posts on the retention. J Oral Rehabil 2002;29:28-34.
Yang H-S, Lang LA, Molina A, Felton DA. The effects of dowel design and load direction on dowel-and-core restorations. J Prosthet Dent 2001;85:558-67.
Raiden G, Gendelman H. Effect of dowel space preparation on the apical seal of root canal fillings. Dent Traumatol 1994;10:109-12.
Braga NMA, Paulino SM, Alfredo E, Sousa-Neto MD, Vansan LP. Removal resistance of glass-fiber and metallic cast posts with different lengths. J Oral Sci 2006;48:15-20.
Christel P, Meunier A, Heller M, Torre J, Peille C. Mechanical properties and short-term in vivo
evaluation of yttrium-oxide-partially-stabilized zirconia. J Biomed Mater Res 1989;23:45-61.
Kwiatkowski SJ, Geller W. A preliminary consideration of the glass-ceramic dowel post and core. Int J Prosthodont 1989;2:51-5.
Al-harbi F, Nathanson D. In vitro
assessment of retention of four esthetic dowels to resin core foundation and teeth. J Prosthet Dent 2003;90:547-55.
Kakehashi Y, Lüthy H, Naef R, Wohlwend A, Schärer P. A new all-ceramic post and core system: Clinical, technical, and in vitro
results. Int J Periodontics Restorative Dent 1998;18:586-93.
Aurelio IL, Marchionatti AME, Montagner AF, May LG, Soares FZ. Does air particle abrasion affect the flexural strength and phase transformation of Y-TZP? A systematic review and meta-analysis. Dent Mater 2016;32:827-45.
Fonseca RG, de Oliveira Abi-Rached F, Reis JMdSN, Rambaldi E, Baldissara P. Effect of particle size on the flexural strength and phase transformation of an airborne-particle abraded yttria-stabilized tetragonal zirconia polycrystal ceramic. J Prosthet Dent 2013;110:510-4.
Bottino MA, Baldissara P, Valandro LF, Galhano GA, Scotti R. Effects of mechanical cycling on the bonding of zirconia and fiber posts to human root dentin. J Adhes Dent 2007;9:327-31.
Lamichhane A, Xu C, Zhang F-q. Dental fiber-post resin base material: A review. J Adv Prosthodont 2014;6:60-5.
Macedo VC, e Silva ALF, Martins LRM. Effect of cement type, relining procedure, and length of cementation on pull-out bond strength of fiber posts. J Endod 2010;36:1543-6.
Innella R, Autieri G, Ceruti P, Gassino G. Relation between length of fiber post and its mechanical retention. Minerva Stomatol 2005;54:481-8.
Nissan J, Dmitry Y, Assif D. The use of reinforced composite resin cement as compensation for reduced post length. J Prosthet Dent 2001;86:304-8.
Borer RF, Briffo LA, Haddix JF. Effect of dowel length on the retention of 2 different prefabricated posts. Quintessence Int 2007;38:e164-8.
de Souza NC, Marcondes ML, da Silva D, Borges GA, Júnior LB, Spohr AM. Relined fiberglass post: Effect of luting length, resin cement, and cyclic loading on the bond to weakened root dentin. Oper Dent 2016;41:e174-e82.
Macedo VC, Souza NA, Faria e Silva AL, Cotes C, da Silva C, Martinelli M, et al
. Pullout bond strength of fiber posts luted to different depths and submitted to artificial aging. Oper Dent 2013;38:E128-E33.
e Silva ALF, Casselli DSM, Ambrosano GMB, Martins LRM. Effect of the adhesive application mode and fiber post translucency on the push-out bond strength to dentin. J Endod 2007;33:1078-81.
Gül EB, Atala MH, Eşer B, Polat NT, Asiltürk M, Gültek A. Effects of coating with different ceromers on the impact strength, transverse strength and elastic modulus of polymethyl methacrylate. Dent Mater J 2015;34:37-97.
Ishigami K, Chiba A, Ohki K, Yokota S, Takeda T. Basic physical properties of Conquest, a high strength tooth crown resin. J Jpn Prosthodont Soc 1996;40:24-8.
Choudhary S, Begum Z, Choudhary P, Tripathi S. Comparative evaluation of retention of prefabricated and conventional cast post: An in vitro
study. J Int Soc Prev Community Dent 2014;4:87-91.
Goracci C, Raffaelli O, Monticelli F, Balleri B, Bertelli E, Ferrari M. The adhesion between prefabricated FRC posts and composite resin cores: Microtensile bond strength with and without post-silanization. Dent Mater 2005;21:437-44.
[Figure 1], [Figure 2], [Figure 3], [Figure 4]